Download presentation

Presentation is loading. Please wait.

Published byAnnette Downer Modified about 1 year ago

1
Modelling of Defects DFT and complementary methods Tor Svendsen Bjørheim PhD fellow, FERMiO, Department of Chemistry University of Oslo NorFERM-2008, 3 rd -7 th of October 2008

2
Outline Background / Introduction DFT Theory DFT calculations in practice Case studies Supplementary Methods Nudged Elastic Band Molecular Dynamics Monte Carlo approach Summary

3
Introduction to defect modeling Experimental techniques Time consuming Expensive Inconclusive results Supplement with computational studies Condensed systems Mutually interacting particles Described by the full Hamiltonian: Increasingly complex with larger number of electrons (3N variables) Need simplifications! Hartree-Fock DFT

4
DFT - Density Functional Theory

5
Density Functional Theory Ab initio ground state theory Basic variable electron density, n(r) n(r) depends only on the three spatial variables Hohenberg-Kohn theorems (1964): For a system of interacting particles in an external potential, the external potential and hence the total energy is a unique functional of n(r) The ground state energy can be obtained variationally; the density that minimizes the total energy is the exact ground state density Problem: kinetic energy of the electrons… Practical use: Kohn-Sham approach (1965) Introduce a reference system of non-interacting particles (with the same n(r)) Kinetic energy easily determined: Functional = Function of a function

6
Total energy: E xc : Need to determine the orbitals of the reference system Kohn-Sham equations: Kohn-Sham potential: Depends on the electron density Can not be solved directly Self consistent solutions using iterative schemes Kohn-Sham approach In principle exact Do not know the form of E XC Approximate Modern DFT: new and improved E XC

7
Simplest approach: Local Density Approximations - LDA Assume E xc equal to E xc in a homogeneous electron gas: Locally constant electron density Systems with slowly varying electron densities Inadequate for systems with quickly varying electron densities Improvements: Generelized-Gradient Approximations (GGA) Include gradients of the electron density at each point E.g. GGA-PW91 and GGA-PBE Problems: Band gaps and Van der Waals forces….. Exchange-Correlation Functionals

8
DFT calculations in practice Real solids ~10 23 atoms Huge number of wave functions.. Need further simplifications! Popular approach: plane waves Periodically repeating unit cell Bloch’s theorem: Finite number of wave functions over an infinite number of k-points in the 1. Brillouin Zone! K-point sampling Electronic states at a finite number of k-points Finite number of wave functions at a finite number of k-points in the 1. Brillouin Zone! K-mesh needs to be chosen carefully

9
Defects in solids Solids with one or more defects Aperiodic systems Bloch’s theorem can not be applied Can not use plane wave basis sets Introduce the concept of a periodically repeating supercell Supercell method Defects in a ’box’ consisting of n unit cells Define the supercell with the defect as the new unit cell Periodic boundaries 3D periodic ordering of defects Typical size: <500 atoms Surfaces/interfaces & molecules

10
Finite-Cluster approach Defects in finite atomic clusters No interaction with defects in neighboring unit cells Avoid surface effects: large clusters Green’s Function Embedding Technique Purely mathematical Defect regions embedded in known DFT Green’s function of bulk Ideal for studies of isolated defects (in theory) Numerically challenging….. Alternative approaches

11
Structural studies Defect positions Locate global minimum E.g. proton positions Local arrangement around isolated defects E.g. local displacements in ferroelectrics

12
Thermodynamics Formation energy of isolated point defects: Defects that change the composition: Total energies and a set of chemical potentials E.g. isolated protonic defects & oxygen vacancies: Formation: Formation energy: Effective defect concentration Supercell size (unit cells) Atmospheric conditions - Thermodynamic tables - Fermi level:

13
Formation energies not directly comparable with experimental results DFT = ground state = 0 K! Chemical potential of the electrons Combine to e.g. hydration: E.g. hydration of AZrO 3 perovskites Increasing stability in orthorhombic perovskites ∆H hydr (DFT) reproduce experimental trends (eV) (kJ/mol) CaZrO SrZrO PbZrO BaZrO

14
Defect levels Transition between charge states: E f (q/q’) Experimentally: DLTS Determine the preferred charge state of defects In supercell calculations: Determine Δ E f for all charge states Δ E f for all Fermi level positions Most stable: charge state with lowest Δ E f

15
Possibilities: Protons, neutral hydrogen & hydride ions Transition levels ε(0/-), ε(+/0), ε(+/-) ZnO [2] ε(+/-) above CBM H: shallow donor Only stable LaNbO 4 [3] ε(+/-) 1.96 eV below CBM favorable at high Fermi levels n-type LaNbO 4 : dominated conductivity? [2] C.G. Van de Walle and J. Neugebauer, Nature (2003), 423 [3] A. Kuwabara, Private Communication, (2008) Hydrogen in semiconductors

16
Overall dominating defect (concentration-wise) Need to calculate all possible defects LaNbO 4 [3] Interstitial oxygen dominates at high Fermi levels (0 K!) [3] A. Kuwabara, Private Communication, (2008)

17
When DFT fails… In defect calculations: band gaps Heavily underestimated Both LDA/GGA functionals Affects: Defect levels Defect formation energies Correction: scissor operation! Shift the conduction band Align E g (DFT) and E g (EXP) Donor type defects follow CB Correct formation energies Alternative: hybrid or semi-empirical functionals / eV BaZrO PbZrO ZnO1.93.4

18
Complementary methods

19
Nudged Elastic Band Method Method for studying transition states: Saddle points Minimum Energy Paths (MEP) Know initial and final states Local/global minima Obtained by total energy calculations (DFT) Reaction path Divided into ’images’ (< 20) Image = ‘ snapshots’ between initial and final states Equidistant images - connected by ’springs’ Optimize each image (DFT+forces) MEP Chosen images not saddle points interpolate

20
Proton transport in LaPO 4 [5] Proton transport in LaPO 4 using NEB+DFT (VASP) Saddle points: Jump rates: Determine dominating transport mechanism Diffusion and conductivity: Proton transport processes: Rotation around oxygen Oscillatory motion Intra-tetrahedral jumps Inter-tetrahedral jumps [5] R. Yu and L. C. De Jonghe, J. Phys. Chem. C 111 (2007) 11003

21
Intratetrahedral jumps: High energy barrier Intertetrahedral jumps: Two tetrahedrons Lower energy barrier Intertetrahedral jumps: Three tetrahedrons Even lower energy barrier Experimentally: eV

22
Molecular Dynamics Used to simulate time evolution of classical many-particle systems Obey the laws of classical mechanics Condensed systems: Classical particles moving under influence of an interaction potential, V(R 1,…,R N ) Forces on the ions: MD algorithms: Discretize equation of motion Trajectories: stepwise update positions and velocities

23
Interionic interactions: Model potential vs. first-principles Model potential Parameterized to fit experimental or first principles data Advantages Possible to treat large systems Long time evolution Disadvantages Inaccurate potentials Poor force representation First-principles First-principles electronic structure calculation (e.g. DFT) at each ionic step Advantages: Accurate forces Realistic dynamic description Disadvatages Computationally demanding Small systems (~100 ions) Short time periods (~ps) Good statistical accuracy Poor statistical accuracy..

24
Monte-Carlo approach Loosely described: Statistical simulation methods Conventional methods (MD): Discretize equations describing the physical process E.g. equations of motion Monte-Carlo approach Simulate the physical process directly No need to solve the underlying equations Requirement: process described by probability distribution functions (PDF) Average results over the number of observations Proton diffusion Jump frequency and PDF:

25
Summary Many different computational approaches Systematic trends Fundamental processes Predict defect properties of real materials Combine different methods

26
Acknowledgements Akihide Kuwabara Espen Flage-Larsen Svein Stølen Truls Norby Colleagues at the Solid State Electrochemistry group in Oslo Thank You !!

27
Thank You!

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google